Standard Practice for Petrographic Examination of Hardened Concrete
This practice outlines the standard procedures for performing petrographic examination of hardened concrete samples. The samples examined may be taken from concrete constructions, that is, all sorts of objects, units, or structures that have been built of hydraulic cement concrete. They may also be concrete products or portions thereof, or concrete or mortar specimens that have been exposed in natural environments or simulated service conditions, or subjected to laboratory tests. This practice applies to samples of all types of hardened hydraulic-cement mixtures, including concrete, mortar, grout, plaster, stucco, terrazzo, and the like. The equipments generally used for specimen preparation are diamond saw, cutting lubricant, horizontal lap wheels, free abrasive machine, polishing wheel, hot plate or oven, prospector's pick and/or bricklayer's hammer, abrasives, plate-glass squares, suitable media, and microscope slides. For specimen examination, the equipments needed are stereomicroscope, dollies, petrographic or polarizing microscope, metallographic microscope, eyepiece micrometer, stage micrometer, microscope lamps, needleholders and points, bottles with droppers, assorted forceps, lens paper, refractometer, and immersion media. Appropriate procedures for the sampling, preparation, and examination of specimens are detailed methodically.
1.1 This practice outlines procedures for the petrographic examination of samples of hardened concrete. The samples examined may be taken from concrete constructions, they may be concrete products or portions thereof, or they may be concrete or mortar specimens that have been exposed in natural environments, or to simulated service conditions, or subjected to laboratory tests. The phrase “concrete constructions” is intended to include all sorts of objects, units, or structures that have been built of hydraulic cement concrete.
Note 1: A photographic chart of materials, phenomena, and reaction products discussed in Sections 8 – 13 and Tables 1–6 are available as Adjunct C856 (ADJCO856).
1.2 The petrographic procedures outlined herein are applicable to the examination of samples of all types of hardened mixtures, including concrete, mortar, grout, plaster, stucco, terrazzo, and the like. In this practice, the material for examination is designated as “concrete,” even though the commentary may be applicable to the other mixtures, unless the reference is specifically to media other than concrete.
1.3 The purposes of and procedures for petrographic examination of hardened concrete are given in the following sections:
Qualifications of Petrographers and Use of Technicians
Purposes of Examination
Selection and Use of Apparatus
Examination of Samples
Visual and Stereomicroscope Examination
Polarizing Microscope Examination
1.4 The values stated in inch-pound units are to be regarded as the standard. The SI units in parentheses are provided for information purposes only.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use. A specific hazard statement is given in 18.104.22.168.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
Formato físico y digital
Nota: Precios sin IVA ni gastos de envío
Descuentos no acumulables
Añadir a la cesta